CrystallizationofMalonicandSuccinicAcidsonSAMs ... grown on the SAMs of HS(CH 2) 10CO 2H and HS(CH...
Embed Size (px)
Transcript of CrystallizationofMalonicandSuccinicAcidsonSAMs ... grown on the SAMs of HS(CH 2) 10CO 2H and HS(CH...
14002 DOI: 10.1021/la902739q Langmuir 2009, 25(24), 14002–14006Published on Web 09/21/2009
© 2009 American Chemical Society
Crystallization ofMalonic and Succinic Acids on SAMs: Toward theGeneral Mechanism of Oriented Nucleation on Organic Monolayers†
Boaz Pokroy,‡ Victoria Fay Chernow, and Joanna Aizenberg*
School of Engineering and Applied Sciences, Department of Chemistry and Chemical Biology, Harvard University, Cambridge, Massachusetts 02138. ‡Current address: Department of Materials Engineering, Israel
Institute of Technology, Haifa 32000, Israel.
Received July 25, 2009. Revised Manuscript Received September 2, 2009
Self-assembled monolayers (SAMs) were shown to induce very specific oriented growth of simple organic and inorganic crystals. Here we present a detailed study of themechanism bywhich SAMs control the oriented nucleation by examining a more complex case of crystallization of bifunctional organic molecules. Malonic and succinic acids were grown on the SAMs of HS(CH2)10CO2H and HS(CH2)11CO2H supported on gold films. Each SAM induced a very controlled, specific orientation of the crystals. The preferred nucleating planes always exhibited an alignment of one of the carboxylic acid groups in the molecules of the growing crystal with the carboxylic acid groups on the surface of the SAMs. These results suggest that the translation of the structural information through the interface occurs by stereochemical registry such that the functional groups in the SAM play the role of an oriented surrogate layer for the nucleating crystal. These findings are very important to the understanding of the underlying principles by which various organic surfaces;and most probably also biological templates;control the crystallization process.
An understanding of crystal nucleation and growth and the ability to control the crystallization process are extremely im- portant in many aspects of science and technology.1 This control is usually achieved by the use of inorganic crystalline substrates that induce nucleation via epitaxy.2 Successful crystallization on these substrates is dependent on the ability to engineer the interface that provides a good lattice match between the substrate and a certain crystallographic plane of the overgrowing crystalline material. For this purpose, much effort is invested in the devel- opment of new, low-mismatch epitaxial inorganic materials that direct the growth of the nascent crystalline phase in specific crystallographic orientations and thus control the optical, elec- tronic, mechanical, biochemical, and catalytic properties. How- ever, the high symmetries of the surfaces in the substrate inorganic crystals put severe limitations on the resulting crystal orientations, especially when symmetry breaking is required to ensure the nucleation and stabilization of a low-symmetry phase and its growth in an arbitrary crystallographic direction.3
The formation of a variety of crystalline materials in organ- isms, however, is templated by bioorganic substrates that exert very high control over crystal nucleation and growth, including polymorph selection, crystallographic orientation, defect distri- bution, and patterning.4 In the materials community, there is a growing appreciation of the potential of biomimetic approaches to crystallization when organic surfaces are used as crystallization
templates to control the formation of both organic and inorganic materials. Several types of biomimetic structured organic substrates have been employed for such purposes. Prominent examples include organic monolayers such as Langmuir mono- layers5,6 and self-assembled monolayers (SAMs).7-15 Alka- nethiol-based SAMs are known to form very ordered 2D crystals on coinage metals.16,17 These SAM organizations have beenwell characterized in terms of their 2D lattice and the tilt and cant angles of the alkyl chains.18-22 The lattice parameters of the surface can be controlled to a certain extent by choosing the appropriate thiol/metal combination. In addition, the use of ω- functionalized SAMsallows for fine-tuning the surface chemistry, charge, polarity, and orientation of the terminal groups. These SAMs have been shown to be extremely potent in inducing the
† Part of the “Langmuir 25th Year: Self-assembled monolayers, synthesis, characterization, and applications” special issue. *Corresponding author. E-mail: firstname.lastname@example.org. (1) Scheel, H. J., Capper, P., Eds.; Crystal Growth Technology: From Funda-
mentals and Simulation to Large-Scale Production; Wiley-VCH: Weinheim, Germany, 2008; p 505. (2) Herman, M. A.; Richter, W.; Sitter, H. Epitaxy: Physical Principles and
Technical Implementation; Springer-Verlag: Berlin, Germany, 2004; p 522. (3) Georgakilas, A.; Panayotatos, P.; Stoemenos, J.; Mourrain, J. L.; Christou,
A. J. Appl. Phys. 1992, 71, 2679–2701. (4) Lowenstam, H. A.; Weiner, S.On Biomineralization; Oxford University Press:
New York, 1989.
(5) Landau, E.M.; Popovitz-biro, R.; Levanon,M.; Leiserowitz, L.; Lahav,M.; Sagiv, J. Mol. Cryst. Liq. Cryst. 1986, 134, 323–335.
(6) Arkadi, L. L.; Suresh, V.; David, L. K.; Stephen, M. Adv. Mater. 1997, 9, 124–127.
(7) Flath, J.; Meldrum, F. C.; Knoll, W. Thin Solid Films 1998, 329, 506–509. (8) Meldrum, F. C.; Flath, J.; Knoll, W. J. Mater. Chem. 1999, 9, 711–723. (9) Heywood, B. R.; Mann, S. Adv. Mater. 1994, 6, 9–20. (10) Aizenberg, J.; Black, A. J.; Whitesides, G. M. J. Am. Chem. Soc. 1999, 121,
4500–4509. (11) Aizenberg, J.; Black, A. J.; Whitesides, G. M. Nature 1999, 398, 495–498. (12) Han, Y. J.; Aizenberg, J. Angew. Chem., Int. Ed. 2003, 42, 3668–3670. (13) Briseno, A. L.; Aizenberg, J.; Han, Y. J.; Penkala, R. A.; Moon, H.;
Lovinger, A. J.; Kloc, C.; Bao, Z. A. J. Am. Chem. Soc. 2005, 127, 12164–12165. (14) Dabros, M.; Thalladi, V. R. Chem. Commun. 2007, 24, 2476–2478. (15) Cox, J. R.; Dabros, M.; Shaffer, J. A.; Thalladi, V. R. Angew. Chem., Int.
Ed. 2007, 46, 1988–1991. (16) Ulman, A. An Introduction to Ultrathin Organic Films: From Langmuir-
Blodgett to Self - Assembly; Academic Press: San Diego, CA, 1991. (17) Love, J. C.; Estroff, L. A.; Kriebel, J. K.; Nuzzo, R. G.; Whitesides, G. M.
Chem. Rev. 2005, 105, 1103–1169. (18) Laibinis, P. E.; Whitesides, G. M. J. Am. Chem. Soc. 1992, 114, 1990–1995. (19) Nuzzo, R. G.; Dubois, L. H.; Allara, D. L. J. Am. Chem. Soc. 1990, 112,
558–569. (20) Fenter, P.; Eisenberger, P.; Liang, K. S. Phys. Rev. Lett. 1993, 70, 2447–
2450. (21) Chaudhuri, A.; Lerotholi, T. J.; Jackson, D. C.; Woodruff, D. P.; Robert,
G. J. Phys. Rev. B 2009, 79, 195439. (22) Fang-Sen, L.; Wancheng, Z.; Quanmin, G. Phys. Rev. B 2009, 79, 113412.
DOI: 10.1021/la902739q 14003Langmuir 2009, 25(24), 14002–14006
Pokroy et al. Article
very specific oriented nucleation of a variety of crystalline materials.7-15
We have previously proposed that the orientation in these systems is not governedby the epitaxialmatchbetween the lattices of the SAM and the crystal nucleation plane, as observed in the traditional inorganic substrates, but rather by their stereochemi- cal registry10,12,13;a spatial match between the orientation of the SAM’s functional groups and that of a certain moiety (or ion) in the nucleated crystal. This mechanism was demonstrated to operate in templating the oriented growth of both inorganic and organic crystals. In particular, the growth of calcium carbo- nate on carboxylate-terminated SAMs was shown to favor calcite orientations with a perfect stereomatch and alignment of the carboxylates in the SAM with the carbonates in calcite, with highly mismatched lattices.10,12 Similarly, anthracene crystals grown on terphenylthiol SAMs exhibited preferred orientation with anthracenemolecules coaligned with the terphenyl groups in the SAM,13 even though such an orientation leads to a lattice mismatch at the interface.23
Here we study the generality of the proposed mechanism of oriented nucleation at organic surfaces by examining a more complex case of crystallization of bifunctional organic molecules. The importance of understanding the crystallization of such systems arises from the fact that the molecules in the nascent crystalline phase can present more than one orientational match with the interface or more than one matching group, thus allowing one to observe how the system selects or discriminates certain orientations and to derive the underlying basic principles. To this end, we have chosen to study the SAMs-induced crystallization of two carboxylic diacids;malonic acid (HOO- CCH2COOH) and succinic acid (HOOCCH2CH2COOH).Malo- nic acid exhibits a triclinic unit cell with the P1 space group (a= 5.330 Å, b= 5.140 Å, c= 11.250 Å, R= 70�, β= 135.17�, and γ = 85.17�).24 Succinic acid exhibits a monoclinic unit cell with the P21/c space group (a = 5.526 Å, b = 8.881 Å, c = 5.105 Å, and β = 91.49�).25 Both acids have two molecules per unit cell, thus presenting four different orientations of the carboxylic acid groups in the crystalline state. We show that in these complex systems the SAMs induce very controlled oriented growth of the crystals. The preferred nucleating planes always exhibit an align- ment of one of the carboxylic acid groups in the molecules of the growing crystal with the carboxylic acid groups on the surface of the SAMs. These results further confirm that the translation of structural information through the organic interface occurs by stereochemical registry such that the functional endgroups in the SAM play the role of an oriented surrogate layer for the nucleat- ing crystal.
Results and Discussion